Structures of Fe^II^ spin-crossover complexes from synchrotron powder-diffraction data
Dova, Eva; Peschar, René; Sakata, Makoto; Kato, Kenichi; Stassen, Arno F.; Schenk, Henk; Haasnoot, Jaap G.; Acta Crystallographica Section B 60 (2004) 528–538; doi:10.1107/S0108768104015356

data_2102632
_publ_section_title
;
 Structures of Fe^II^ spin-crossover complexes from synchrotron
 powder-diffraction data
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              528
_journal_page_last               538
_journal_paper_doi               10.1107/S0108768104015356
_journal_volume                  60
_journal_year                    2004
_chemical_formula_sum            'C18 H30 B2 Br6 F8 Fe N24'
_chemical_formula_weight         1291.53
_chemical_name_systematic        ' ?'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_audit_creation_method           'from EXP file using GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.106(3)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   12.2832(6)
_cell_length_b                   18.0705(15)
_cell_length_c                   10.4767(3)
_cell_measurement_temperature    300
_cell_volume                     2325.4(2)
_computing_structure_refinement  GSAS
_diffrn_measurement_device_type  'Debye Scherrer'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.999995
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_refine_ls_goodness_of_fit_all   6.38
_refine_ls_matrix_type           full
_refine_ls_number_parameters     184
_refine_ls_number_restraints     145
_refine_ls_shift/su_max          0.64
_refine_ls_shift/su_mean         0.05
_cod_data_source_file            na5021.cif
_cod_data_source_block           LAST_publ
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (175
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (88 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_cell_measurement_temperature' value '300 K' was changed to '300' -
the value should be numeric and without a unit designator.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_cell_measurement_temperature' value '300 K' was changed to '300' -
the value should be numeric and without a unit
designator.

'_geom_bond_publ_flag' value 'N' changed to 'n'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29 (175
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (88 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        2325.44873
_cod_database_code               2102632